DOI: 10.15632/jtam-pl.55.1.129

**AN ENERGY-BASED METHOD IN PHENOMENOLOGICAL DESCRIPTION**
**OF MECHANICAL PROPERTIES OF NONLINEAR MATERIALS UNDER**

**PLANE STRESS**

Tadeusz Wegner, Dariusz Kurpisz

*Poznan University of Technology, Institute of Applied Mechanics, Poznań, Poland*
*e-mail: [email protected]*

A method based on energy is a very useful tool for description of mechanical properties of materials. In the current paper, on the base of geometrical interpretation of a deformation process, the strain energy density function for isotropic nonlinear materials has been con-structed. On account of hydrostatic interpretation of the volumetric deformation, the elastic part of energy has been extracted. The initiation of the damage process due to plastic ﬂow of the material under plane stress has been determined and the stability conditions have been formulated by using in the stability analysis the strain energy density function in addition to Sylvester’s theorem and assumption of zero volume change during pure plastic deformations. This concept is an original part of the work and continuation of the investigations previously carried out by Wegner and Kurpisz. The theoretical investigations have been illustrated on the example of aluminium.

*Keywords:* energy-based method, nonlinear material, phenomenological description, strain
energy density function, Sylvester’s theorem

**1.** **Introduction**

The phenomenological description of mechanical properties of nonlinear materials is interesting
due to possibility of its application to real engineering structures. The knowledge about
mecha-nisms of deformation under the inﬂuence of external loads and the relations between them can
be very important in the design process. There is a lot of publications devoted to the modelling
of mechanical properties based both on the ground of microstructure relations in the material
*(multi-scale modelling methods), see for example Silva et al. (2007), Terada et al. (2008), Speirs*
*et al. (2008), or on a phenomenological concept, see for example Wegner (2000, 2005). Because*
we consider mechanical properties on the base of a real experiment in which the object
(mate-rial sample) and measured properties are usually in macro-scale, so using the phenomenological
method as the way of modelling of the process, which is directly connected with the
experi-ment, is recommended. From this point of view, very interesting are methods based on energy,
which were used by Petryk (1985, 1991), Schroder and Neﬀ (2003), Wegner (2000, 2005, 2009)
*and Dargazany et al. (2012). Here, the necessary tool of description of mechanical properties*
of materials is the strain energy density function. It can be introduced in many diﬀerent ways,
for example as a direct function of invariants of the deformation state, see Wegner (1999, 2009)
and Schroder and Neﬀ (2003) or on the base of geometrical interpretation of the deformation
process, see Wegner and Kurpisz (2009). Wegner and Kurpisz (2013), using a phenomenological
approach and basing on the strain energy density function, investigated the damage process of
a metal foam.

Material damage as a dissipative mechanism described in form of free energy per unit volume
*considered as a thermodynamic potential was taken into account by Cimetiere et al. (2005). The*

authors, in a major way, split the energy into two parts. The ﬁrst is an elastic (reversible) part, whereas the second (dissipative) includes, among others, the hardening eﬀect. Because each of these two parts depends on internal variables, so the internal variables inﬂuence the damage threshold.

Gajewska and Maciejewska (2005) investigated the inﬂuence of internal restrictions (con-nected with the type of the material, for example isotropic or anisotropic one) in form of limit conditions based on energy of anisotropic materials. Such conditions can be interpreted as diﬀe-rent yield conditions. It was shown that as long as the energy scalar product was deﬁned properly in the elastic range, the limit condition having the energy-based interpretation could be found. A much more interesting case takes place when we have nonlinear-elasticity, what implies the necessity of modiﬁcation of the limit condition.

In the further part of the current paper, on the base of geometrical interpretation, the strain energy density function of a nonlinear material will be introduced and used for formulation of stability conditions due to the damage process, what is an alternative point of view to that presented by Gajewska and Maciejewska (2005).

**2.** **Geometrical interpretation of the deformation state – the basic equation**

To introduce a geometrical interpretation of the deformation process, let us take into account the following assumptions:

*• The material is isotropic and nonlinear, so the mechanical properties are the same in all*
directions, but the relations between stress and strain can not be described in form of
classic Hook’s law (for linear materials).

*• The loading process is static, which means that dynamic eﬀects can be neglected.*
*• The dissipated part of energy includes thermal and plastic deformation energy.*
*• The material is under plane stress.*

*• The longitudinal deformation coeﬃcient is a function of the deformation state due to*
nonlinear properties of the material.

*• The principal stress and strain directions are the same due to material isotropy.*

*Every deformation process can be interpreted as a deformation path C, which is located in*
space of principal deformation state components. Every point of such path is one deformation
state. So a change of deformation due to a change of external loads (change of principal stress
components) implies a displacement along the path

*C : εi= εk _{i}t* for

*i = 1, 2, 3*(2.1)

*where εk*

*i* *are the ﬁnal deformation state components, and t ∈ T = h0, 1i is a parameter.*

The relation between stress and strain in every point of the deformation path takes the form of generalized Hook’s law

*ε*1=
*σ*1*(t)*
e
*E(ε*1)
*−*e*v(ε*2)
*σ*2*(t)*
e
*E(ε*2)
*−*e*v(ε*3)
*σ*3*(t)*
e
*E(ε*3)
*ε*2=
*σ*2*(t)*
e
*E(ε*2)
*−*e*v(ε*1)
*σ*1*(t)*
e
*E(ε*1)
*−*e*v(ε*3)
*σ*3*(t)*
e
*E(ε*3)
*ε*3=
*σ*3*(t)*
e
*E(ε*3)
*−*e*v(ε*1)
*σ*1*(t)*
e
*E(ε*1)
*−*e*v(ε*2)
*σ*2*(t)*
e
*E(ε*2)
(2.2)

Fig. 1. Deformation paths for a triaxial and plane stress state in a material

where longitudinal and transversal deformation coeﬃcients follow from experimental
*characte-ristics σ(ε), εt(ε) (εt* is transversal deformation) obtained from a uniaxial tension test and take
respectively the form

e

*E(ε) =* *σ*

*ε* *v(ε) = −*e
*εt*

*ε* (2.3)

*Because both stress and strain are changeable (along path Cf _{) in time t ∈ h0, 1i of the}*

*deformation process, then the density of deformation work from the initial state εi*

*= 0 for t = 0*

*to the ﬁnal state εi*

*= εki*

*for t = 1 can be expressed as*

*WC(εk*_{1}*, εk*_{2}*, εk*_{3}) =
Z
*Cf*
3
X
*i*=1
*σi* *dεi* =
1
Z
0
3
X
*i*=1
*σi(t)ε′i(t) dt* (2.4)

*where on the basis of (2.2) for i = 1, 2, 3*

*σi(t) =E(εi)*e
*εi* Q3
*l*=1
[1 +e*v(εl)] + [1 +*e*v(εi)]*P3
*l*=1e
*v(εl)(εl _{− ε}i*) +1+

_{e}

*e*

_{v}*)*

_{(ε}v(εi*i*) 3 Q

*l*=1e

*v(εl)*P3

*l*=1

*εl*! 3 Q

_{− 3ε}i*l*=1 [1 +e

*v(ε*e

_{l)] − [1 +}*v(εi*)]2 3 P

*l*=1e

*v(ε*e

_{l) −}v(ε*i*) +

_{e}

*2*

_{v}_{(ε}*i*) 3 Q

*l*=1e

*v(εl*) ! (2.5)

*In particular, if we assume the plane stress in plane 1O2, then the stress components in the*third direction are equal zero, and relations (2.4) and (2.5) simplify respectively to

*WC(εk*_{1}*, εk*_{2}) =
Z
*Cf*
2
X
*i*=1
*σidεi* =
1
Z
0
2
X
*i*=1
*σi(t)ε′*
*i(t) dt* (2.6)
and
*σ*1*(t) =E(ε*e 1)
*ε*1*+ ε*2*v(ε*e 2)
*1 −*e*v(ε*1)e*v(ε*2)
*σ*2*(t) =E(ε*e 2)
*ε*2*+ ε*1e*v(ε*1)
*1 −v(ε*e 1)*v(ε*e 2)
(2.7)

The strain component in the passive (third) direction takes the form
*ε*3 *= −*e*v(ε*1) *ε*1*+ ε*2*v(ε*e 2)
*1 −*e*v(ε*1)e*v(ε*2) *−*e
*v(ε*2) *ε*2*+ ε*1*v(ε*e 1)
*1 −v(ε*e 1)*v(ε*e 2)
(2.8)
In the geometrical interpretation, function (2.6) speciﬁes the values of deformation work
density (2.4), which are deﬁned in the space of three-dimensional deformation to present a
strain energy density distribution function plot (Fig. 5) along section surface (2.8).

**3.** **Extraction of the volumetric part of energy**

Let us consider purely volumetric deformations. Such type of deformations takes place if a material is under inﬂuence of hydrostatic pressure. The relation between deformation state components and stress state components according to hydrostatic pressure takes the form

*εV*_{1} = *ks*
e
*E(εV*
1)
*−v(ε*e *V*_{2}) *ks*
e
*E(εV*
2)
*−v(ε*e *V*_{3}) *ks*
e
*E(εV*
3)
*εV*_{2} = *ks*
e
*E(εV*
2)
*−v(ε*e *V*_{1}) *ks*
e
*E(εV*
1)
*−v(ε*e *V*_{3}) *ks*
e
*E(εV*
3)
*εV*
3 =
*ks*
e
*E(εV*
3)
*−v(ε*e *V*
1)
*ks*
e
*E(εV*
1)
*−v(ε*e *V*
2)
*ks*
e
*E(εV*
2)
(3.1)

*where s ∈ T and hence, due to symmetry*

*εV*_{1} *= εV*_{2} *= εV*_{3} *= εV* (3.2)

*where εV* _{satisﬁes the equation}
*εV* = *1 − 2*e*v(ε*

*V*_{)}

e

*E(εV*_{)} *ks = β(s)* (3.3)

*and s is a non-dimensional parameter: the ratio of hydrostatic pressure to the basic value k,*
*ks is the current value of hydrostatic pressure.*

The above relation does not provide the information about the connection between the
*current value of deformation (point of path C) and its volumetric part (point of path CV*), see
the picture below.

*Fig. 2. Relation between the deformation path C and the path due to pure volumetric deformation CV*

To determinate this relation, we have to take into account two analytical descriptions of a volume change in an elementary piece of the material.

The ﬁrst way
*∆V*
*V*0
=
3
Y
*i*=1
*[1 + εi(t)] − 1* (3.4)

*where ε*1*(t), ε*2*(t) and ε*3*(t) are deformation components of the path C.*

The second way explores hydrostatic pressure
*Θ =* *∆V*
*V*0
=
3
Y
*i*=1
*[1 + β(s)] − 1 = [1 + β(s)]*3*− 1* (3.5)

*where Θ is the relative volume change.*

After comparison of the right-hand sides of equations (3.4) and (3.5), we receive
*s = h(t) = β−1* 3
v
u
u
tY3
*i*=1
*[1 + εi _{(t)] − 1}*
!
(3.6)
and after substitution into (3.3)

*εV* = 3
v
u
u
tY3
*i*=1
*[1 + εi _{(t)] − 1}* (3.7)

Hence, we can write that
*WCV* =
Z
*CV*
*σ*1*dεV*1 +
Z
*CV*
*σ*2 *dεV*2 +
Z
*CV*
*σ*3 *dεV*3 =
3
X
*i*=1
Z
*CV*
*σidεV* (3.8)

*where σi* *(i = 1, 2, 3) are solutions to the system of equations (2.2) given in form (2.5).*

**4.** **Stability conditions for the material under plane stress**

The material is in the stable state of equilibrium if every change of the deformation state needs work to be done by external loads. So, in other words, we say about material stability when the strain energy density function is convex. In an analytical form, it can be written as

*δ*2*WC* =
3
X
*i*=1
3
X
*j*=1
*∂*2*WC*
*∂εk*
*i∂εkj*
*δεk _{i}δεk_{j}*

*> 0*(4.1)

*where δ*2 _{denotes the second order variation of the function W}C_{.}

*In the case of plane stress, the deformation work WC* _{can be interpreted as a function of two}
deformation state components, however from the other side, the strain energy density depends
on three deformation state components and the sign of its second order variation of the strain
energy is strictly connected with the three variation increments of deformation state components.
Hence, on the base of Sylvester’s theorem, we receive

*∂*2*WC*
*∂(εk*
1)2
*∂*2*WC*
*∂εk*
1*∂εk*2
*∂*2*WC*
*∂εk*
1*∂εk*3
*∂*2*WC*
*∂εk*
1*∂εk*2
*∂*2*WC*
*∂(εk*
2)2
*∂*2*WC*
*∂εk*
2*∂εk*3
*∂*2*WC*
*∂εk*
1*∂εk*3
*∂*2*WC*
*∂εk*
2*∂εk*3
*∂*2*WC*
*∂(εk*
3)2
*> 0*
*∂*2*WC*
*∂(εk*
1)2
*∂*2*WC*
*∂εk*
1*∂εk*2
*∂*2_{W}C*∂εk*
1*∂εk*2
*∂*2_{W}C*∂(εk*
2)2
*> 0*
*∂*2_{W}C*∂(εk*
1)2
*∂*2_{W}C*∂εk*
1*∂εk*3
*∂*2*WC*
*∂εk*
1*∂εk*3
*∂*2*WC*
*∂(εk*
3)2
*> 0*
*∂*2_{W}C*∂(εk*
2)2
*∂*2_{W}C*∂εk*
2*∂εk*3
*∂*2*WC*
*∂εk*
2*∂εk*3
*∂*2*WC*
*∂(εk*
3)2
*> 0*
*∂*2*WC*
*∂(εk*
1)2
*> 0*
*∂*2*WC*
*∂(εk*
2)2
*> 0*
*∂*2*WC*
*∂(εk*
3)2
*> 0*
(4.2)

Inequality (4.1) implicates a system of six nonlinear inequalities (4.2) which allow us to draft the region of material stability. Because the plastic deformation leads to permanent loss of the element shape, so very important is the knowledge about material deformation due to plastic ﬂow. This type of phenomenon takes place if during the deformation process, the volume change of an elementary piece of the material is unchanging.

On the basis of (A.15, see Appendix), the second order variation takes the form
*δ*2*WV*= const =
3
X
*i*=1
3
X
*j*=1
*∂*2_{W}C*∂εk*
*i∂εkj*
*−*1
3
3
X
*k*=1
*σk*
3
*√*
*A*1*A*2*A*3
*∂Ai*
*∂εk*
*j*
!
*δεk _{i}δεk_{j}*
=
3
X

*i*=1 3 X

*j*=1

*Bijδεk*(4.3)

_{i}δεk_{j}*where A*1*, A*2*, A*3 *are given as in Appendix (A.3), and σk* are expressed by using (2.5).

Hence, stability assumption (4.3) takes respectively the form

*B*11 *B*12 *B*13
*B*21 *B*22 *B*23
*B*31 *B*32 *B*33
*> 0*
*B*11 *B*12
*B*21 *B*22
*> 0*
*B*11 *B*13
*B*31 *B*33
*> 0*
*B*22 *B*23
*B*32 *B*33
*> 0*
*|B*11*| > 0* *|B*22*| > 0* *|B*33*| > 0*
(4.4)

*In the case of a plane state of stress, so when σ*3 *= 0, εk*3 must to be replaced by relation

(2.8).

**5.** **Example**

As an example of using theoretical investigations, aluminum in plain stress has been taken. The experimental plots of material characteristics are presented in Figs. 3 and 4.

Fig. 3. Experimental relation between stress and strain (in a uniaxial tensile test) and its approximation in the nonlinear range (red line)

However, the precision of approximation of the experimental characteristic between stress
and strain is not suﬃcient for very small (closed to zero) deformations, it is very accurate in the
*range ε ∈ h0.0023; 0.0033i, where there exists danger of the appearance of plastic ﬂow. Because*
in the analytical assessment of the limit surface the second order partial derivatives of the strain

Fig. 4. Experimental plot of transversal deformation coeﬃcient (relation between the ratio of transversal to longitudinal deformation and longitudinal deformation) and its approximation (red line)

energy density function are very important, then much more important is the accuracy of the
*approximation for ε ∈ h0.0023; 0.0033i than for ε ∈ h0; 0.0023i.*

*Analytical approximations of the above characteristics (σ [MPa],* *v(ε) [MPa],*e *E(ε) [MPa])*e
can be written respectively as

*σ = −11100000ε*2*+ 86700ε + 9* for * _{ε ∈ h0; 0.0033i}*
e

*v(ε) =*

*0.317*for

_{ε ∈ h0; 0.0032i}*0.366*

*π*arctan 2

*601εε − 0.0032*

*0.02 − ε*

*+ 0.317*for

*ε > 0.0032*(5.1)

Hence from (2.3)1 and (5.1), we have

e

*E(ε) = −11100000ε + 86700 +* 9

*ε* for *ε ∈ h0; 0.0033i* (5.2)

*The strain energy density function (WC* _{[MJ/m}3_{]) due to (2.5), (5.1) and (5.2) takes the}

form
*WC(εk*_{1}*, εk*_{2}*, εk*_{3}) =
1
Z
0
3
X
*i*=1
*σi(t)ε′i(t) dt =*
1
Z
0
3
X
*i*=1
*σi(t)εki* *dt*
= *a*1*(1 + c*1*) − 3a*1*c*1
*3(1 + c*1*)(1 − 2c*1)
3
X
*i*=1
*(εk _{i}*)3+

*b*1

*(1 + c*1

*) − 3b*1

*c*1

*2(1 + c*1

*)(1 − 2c*1) 3 X

*i*=1

*(εk*)2 +

_{i}*a*1

*c*1

*3(1 + c*1

*)(1 − 2c*1) 3 X

*i*=1

*(εk*)2 3 X

_{i}*l*=1

*εk*+

_{l}*b*1

*c*1

*2(1 + c*1

*)(1 − 2c*1) 3 X

*i*=1

*εk*!2 + 1

_{i}*1 − 2c*1 3 X

*i*=1

*εk*(5.3)

_{i}*where a*1

*= −11100000, b*1

*= 86700, c*1

*= 0.317.*

If we would like to represent and plot in an easy way the strain energy density
func-tion for a plain state of stress, then we have to substitute (on the basis of relafunc-tion (2.8))
*εk*

3 *= −[c/(1 − c)](εk*1 *+ εk*2) into relation (5.4). After transformations, we receive

*WC(εk*_{1}*, εk*_{2}_{) = −36815920[(ε}k_{1})3*+ (εk*_{2})3*] + 431343.3[(εk*_{1})2*+ (εk*_{2})2]

*+ 117.94(εk*_{1} *+ εk*_{2}_{) − 331343284[(ε}k_{1})2*εk*_{2} *+ εk*_{1}*(εk*_{2})2*] + 7764179.1εk*_{1}*εk*_{2} (5.4)
*for εk*

1 *∈ h0; 0.0033i, εk*2 *∈ h0; 0.0033i.*

If we apply relation (5.3) to stability assumptions (4.5) then we receive stability regions shown in Fig. 6.

Fig. 5. The strain energy density function

Fig. 6. Region of stability according to assumptions (4.5) in space of the deformation (a) and the stress (b) components

The above plots are obtained from the major form of stability assumptions (formulated for
*a three-axial state of stress), after substituting the relation εk*

3 *= −[c(1 − c)](εk*1 *+ εk*2), which is

true in the case of plain stress.

**6.** **Conclusions**

*• The strain energy density function is a suﬃcient tool in the description of mechanicals*
properties of nonlinear material and necessary for stability analysis.

*• Extraction of the volumetric part of energy is possible due to hydrostatic interpretation.*
*• The constant volume assumption plays an important role in formulation of stability *

con-ditions due to plastic ﬂow.

*• The limit surfaces are convex (see. Figs. 6) and are comparable with the known limit*
surfaces for linear-elastic materials.

**A.** **Appendix**

The material is in the stable state of equilibrium if every change of current deformation state needs a work by external loads. So, if we take into account a very small ﬂuctuation of the current deformation state in three principal directions then relation (4.1) has to be satisﬁed.

The plastic ﬂow takes place in the case when an increment in volume equals zero, see (Wegner, 2000).

*If l*1*, l*2 *and l*3 are dimensions of an elementary volume piece of the material in an unloaded

state then the ratio of volume change to its virgin state can be written as

*θ =* *∆V*
*V*0
=
3
Q
*i*=1
*(li+ ∆li _{) −}* Q3

*i*=1

*li*3 Q

*i*=1

*li*= 3 Y

*i*=1

*(1 + ε*(A.1) and hence

_{i) − 1}*δθ = δ*"

_{3}Y

*i*=1

*(1 + εi)*# = 3 X

*i*=1

*Aiδεi*(A.2) where

*A*1

*= (1 + ε*2

*)(1 + ε*3)

*A*2

*= (1 + ε*1

*)(1 + ε*3)

*A*3

*= (1 + ε*1

*)(1 + ε*2) (A.3)

*If we take into considerations purely volumetric deformations then εi= εV*_{, which by substitution}
into (A.1) implies

*θ = (1 + εV*)3* _{− 1 ⇒ δθ = 3(1 + ε}V*)2

*δεV*

*=*

_{⇒ δε}V*δθ*

*3(1 + εV*_{)}2 (A.4)

The ﬁrst order variation of the strain energy density function according to plastic ﬂow can be divided as follows

*δW(V = const )= σ*1*δε(V = const )*1 *+ σ*2*δε(V = const )*2 *+ σ*3*δε(V = const )*3

*δε(V = const ) _{i}*

*= δεi− δεV*

(A.5) In the case of the limit surface according to plastic ﬂow, we do not observe a change in the volume, so

*δWV*= const *= δWC _{− δW}CV*

*= δWs*(A.6)

where on the basis of (3.8), we have
*δWCV* =

3 X

*i*=1

*σiδεV* (A.7)

Hence, taking into account (A.4)
*δ*2*WCV* _{=} 1
3
3
X
*i*=1
*σi*
h * _{δ}*2

_{θ}*(1 + εV*

_{)}2

*−*

*2δθδεV*

*(1 + εV*

_{)}3 i (A.8) In the absence of volumetric deformations

*δθ = δεV* = 0 (A.9)
we have
*δ*2*WCV* = 1
3
3
X
*i*=1
*σi*
*δ*2*θ*
*(1 + εV*_{)}2 (A.10)

and after using (A.6)
*δ*2*WV*= const * _{= δ}*2

*2*

_{W}C_{− δ}

_{W}CV_{=}3 X

*i*=1 3 X

*j*=1

*∂*2

_{W}C*∂εi∂εjδεiδεj−*1 3 3 X

*i*=1

*σi*

*δ*2

_{θ}*(1 + εV*

_{)}2 (A.11)

which on the basis of (A.2) gives
*δ*2*WV*= const =
3
X
*i*=1
3
X
*j*=1
*∂*2*WC*
*∂εi∂εj* *−*
1
3
3
X
*k*=1
*σk*
*(1 + εV*_{)}2
*∂Ai*
*∂εj*
!
*δεiδεj* (A.12)

On the grounds of (A.4)

*1 + θ = (1 + εV*)3 * _{⇒ 1 + ε}V* =

*√*3

*1 + θ ⇒ 1 + εV*= 3 v u u tY3

*i*=1

*(1 + εi)*

*⇒ (1 + εV*)2 =p3

*A*1

*A*2

*A*3 (A.13)

The above relation enables us to write (A.12 in an equivalent form
*δ*2*WV*= const =
3
X
*i*=1
3
X
*j*=1
*∂*2*WC*
*∂εi∂εj* *−*
1
3
3
X
*k*=1
*σk*
3
*√*
*A*1*A*2*A*3
*∂Ai*
*∂εj*
!
*δεiδεj* (A.14)
*Acknowledgments*

This study was supported by DS: 02/21/DSPB/3452.

**References**

1. Cimetiere A., Halm D., Marigo J.J., Molines E., 2005, Damage standard models with a
**ﬁxed convex, Archives of Mechanics, 57, 4, 265-276**

2. Dargazany R., Khiem V.N., Nawrath U., Istkov M., 2012, Network evolution model of
ani-sotropic stress softening in ﬁlled rubber-like materials: Parameter identiﬁcation and ﬁnite element
**implementation, Journal of Mechanics and Material and Structures, 7, 8/9, 861-885**

3. Gajewska K., Maciejewska J., 2005, Energy based limit criteria for anisotropic elastic materials
**with constraints, Archives of Mechanics, 57, 2/3, 133-155**

**4. Petryk H., 1985, On the second-order work in plasticity, Archives of Mechanics, 37, 503-520***5. Petryk H., 1991, The energy criteria of instability in the time-independent inelastic solids, *

*Ar-chives of Mechanics***, 43, 4, 519-545**

6. Schroder J., Neff P., 2003, Invariant formulation of hyperelastic transverse isotropy based on
* polyconvex free energy functions, International Journal of Solids and Structures, 40, 401-445*
7. Silva E., Forst C., Li J., Lin X., Zhu T., Yip S., 2007, Multiscale material modelling:

*ca-se studies at the atomistic and electronic structure levels, ESAIM: Mathematical Modelling and*
*Numerical Analysis***, 41, 2, 427-445**

8. Speirs D.C.D., de Souza Neto E.A., Peri’c D., 2008, An approach to the mechanical
*con-stitutive modelling of arterial wall tissue based on homogenization and optimization, Journal of*
*Biomechanics***, 41, 2673-2680**

9. Terada K., Inugai T., Hirayama N., 2008, A method of numerical material testing in
*nonli-near multiscale material analyses (in Japanese), Transactions of the Japan Society of Mechanical*
*Engineering A***, 74, 1084-1094, 2008**

*10. Wegner T., 1999, Methods Based On Energy in Strength of Materials (in Polish), Wydawnictwo*
Politechniki Poznańskiej, Poznań

11. Wegner T., 2000, Surface of limit state in nonlinear material and its relation with plasticity
**condition (in Polish), The Archive of Mechanical Engineering, 47, 3, 205-223**

12. Wegner T., 2005, Mathematical modelling of mechanical properties of materials (in Polish),
*Biuletyn WAT***, LIV, 12, 5-51**

*13. Wegner T., 2009, Modelling Based on Energy in Nonlinear Mechanics of Materials and Structures*
(in Polish), Wydawnictwo Politechniki Poznańskiej, Poznań

14. Wegner T., Kurpisz D., 2009, The conservation energy principle in description of stable and
* unstable states for aluminium, Proceedings in Applied Mathematics and Mechanics, PAMM, 9,*
323-324

15. Wegner T., Kurpisz D., 2013, Phenomenological modeling of mechanical properties of metal
**foam, Journal of Theoretical and Applied Mechanics, 51, 203-214**